# Rev. Esc. Minas vol.67 número2

Alaine Moreira Imbelloni et al.

Mining

Mineração

Nickel ore grinding energy

determination

Determinação energética da moagem do minério

de níquel

Alaine Moreira Imbelloni

Ma, Professora Assistente, CEFET

Araxá, Minas Gerais, Brasil

alaineimbeloni7@gmail.com

José Pedro Silva

Engenheiro Especialista, Samarco Mineração S/A,

Minas Gerais, Brasil

pedro@samarco.com

Carlos Alberto Pereira

Dr. Professor Associado, Universidade Federal de

Ouro Preto, Brasil

pereira@demin.ufop.br

Abstract

This study describes the application of an empirical method to estimate the energy consumption in laboratory of the primary grinding of nickel ore with a speciic

mineralogical texture. This method developed by Donda was previously used in iron

ore from the Iron Quadrangle (Minas Gerais, Brasil) with the same purpose. Through

the grinding test, performed under standard conditions and based on the degree of

liberation and percentage retained on 0.074 mm, it is possible to obtain the energy

consumption for grinding. The results mean a validation of the method with a good

approximation between industrial and laboratory values. In practice the energy consumption is 26.6 kWh/t and through Donda’s method, when using the liberation degree as a parameter, the energy found was 26.8 kWh/t.

keywords: Energy consumption, Nickel ore, Donda’s method

Resumo

Esse estudo descreve a aplicação de um método empírico para estimar, em laboratório, o consumo de energia de moagem primária do minério niquel com uma

textura mineralogica especíica. Esse método desenvolvido por Donda foi usado, anteriormente, em minério de ferro do Quadrilátero Ferrífero (Minas Gerais, Brasil), com

a mesma inalidade. Através do teste de moagem, realizado com condições padronizadas e baseado no grau de liberação e na percentagem retida em 0,074 mm, é possível

obter o consumo de energia de moagem. Os resultados signiicam uma validação do

método com uma boa aproximação entre valores industriais e laboratoriais. Na prática, o consumo de energia é 26,6 kWh/t e, através do método de Donda e usando o grau

de liberação como parâmetro, a energia encontrada foi de 26,8 kWh/t.

Palavras chave: Consumo energético, minério de níquel, metódo de Donda

1. Introduction

In mineral processing plants, the

comminution process is carried out in order to reduce particle size and “unlock”

the mineral species from the gangue,

enabling enrichment of the mineral

content to the desired level in subsequent

concentration processes (WILLS, 2006).

Over the years, various comminution theories were created and were only

concerned with the evaluation of the

relationship between applied energy and

particle reduction. Despite all advances

obtained in the knowledge of grinding, there is a gap about estimating the

speciic energy consumption. The laboratorial energy measurements require

complicated assembly and specialized

labor for the realization of tests. On

other hand, studies in industrial plants

require a large amount of material, take

a long time and have high costs.

Donda (2003) developed a method

to estimate grinding energy consumption

for ball mills using the iron ore concentrate from the Iron Ore Quadrangle

(Minas Gerais, Brazil). Its applicability

has been established for many years for

the re-grinding stage at Samarco Mineração S/A showing a good approximation between industrial and laboratorial

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

185

Nickel ore grinding energy determination

energy values with a range between 0.9

and 1.1 times the value of the s peciic

industrial energy consumption.

This method is an adaptation of the

methodology proposed by Bogren and

Wakeman, at the current Midland Research Center and consists of grindings

using different times with standardized

conditions for ball and ore charge, mill

speed and solid percentage, calculating

the absorbed power per tonne of grinding media through the Rowland equation

for a small mill (diameter until 0.76m).

The use of this method means a simpliication of the laboratory procedures as

being the differentiating factor, since the

tests can be performed in mills built with

minimum care and are not requiring

sophisticated equipment to measure the

energy in the laboratory (Von Krüger,

2004)

Studies about the nickel ore showed

that the liberation of nickel occurs in the

size of ines (0.074 mm) and requires

high power consumption in the primary

grinding. Then, considering the importance of controlling this parameter, this

study’s main goal was to verify the

applicability of the Donda’s method for

ine nickel ore.

was homogenized and quartered. The

grinding tests were performed in a ball

mill utilizing four different times (20,

40, 60 and 80 minutes) with standard

conditions as shown in Table 1. For each

test, the particle size analyses of the feed

and products were determined by wet

screening using Tyler sieves. Chemistry

analysis was performed with samples

of the ground products using optical

microscopy

2. Materials and methods

The experiments were done in the

Laboratory of Mineral Processing at the

University of Ouro Preto using a sample

of nickel ore from the mine of Fortaleza

de Minas belonging to Votorantim Metals Nickel S/A. The initial lot of material

Conditions for the Donda tests

Mill diameter (m)

0.3048

Mill length (m)

0.3048

Ball charge (kg)

30.578

% critical mill speed

70

% of solids

81

Ore charge (kg)

5.623

Media charge

Balls

Ball size distribution (diameter)

Staggered

Table 1

Pre-established conditions for the tests

(Donda, 2003).

(63 to 25 mm)

Using the Rowland equation

(Eq.1), the power was obtained by

multiplying the (kWb) value by the ball

load weight. The speciic energy was

obtained multiplying the power by the

milling time.

(Eq. 1)

Where:

kWb= Kilowatts per tonne of balls

D= Mill diameter inside lifters [m];

VP =Fraction of the mill volume oc-

cupied by the balls mill;

CS = Fraction of critical mill speed.

3. Results

Mineralogical analyses

The Table 2 shows the results of the

mineralogical analyses, which were done

based on the optical microscopy using the

product of the milling test for 60 minutes.

The samples used were composed mainly

of amphibole, pyrrhotite, chlorite, mag-

Mineral

%

Mineral

Amphibole

39

Carbonate

3

Pyrrhotite

20

Biotite

Trace

186

%

Chlorite

12

Chromite

Trace

Pentlandite

11

Pyrite

Trace

Talc + White

Mica/Sericite

6

Pyroxene

Trace

Magnetite

5

Goethite

Trace

Chalcopyrite

3

Ilmenite

Trace

Trace: < 1%

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

netite and pentlandite.

Table 2

Mineralogical analysis

Alaine Moreira Imbelloni et al.

According to the photomicrographs

obtained by optical microscopy with

transmitted light, it was possible to

determine that pentlandite is normally

associated with pyrrohotite as revealed

in Figure 1, which presented a lame of

pentlandite (PDT) in pyrrhotite (PYR).

The Figure 3 shows a pyrrhotite (PYR)

particle with pentlandite (PDT) lames

and a pentlandite (PDT) particle with

pyrrhotite (PYR) edges.

and pyrrhotite (PYR) particle associated

with pentlandite (PDT) as revealed in

Figure 4. For the product of grinding

performed during 80 minutes, note the

free particle composed of pentlandite

(PDT) in Figure 5.

Figure 1

grinding performed during 20 minutes

Figure 2

grinding performed during 40 minutes

After 60 minutes of grinding, it

was possible to notice the presence of a

particle liberated from pentlandite (PDT)

Figure 3

grinding performed during 60 minutes

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

187

Nickel ore grinding energy determination

Figure 4

grinding performed during 20 minutes

Granulometric analysis

Figure 6 shows the graph obtained

from the particle size distribution of

the feed and product for the grinding

tests. The results of P80, calculated as

a function of the test time at 20, 40, 60

and 80 minutes were 0.210 mm; 0.140

mm; 0.125 mm and 0.096 mm.

Figure 5

Particle size distribution

Liberation degree

Calculation of the liberation was

made by Gaudin, obtaining a particle

size equal to 0.125 mm, assuming there

is a variation of up to 3%. Therefore, the

sequence of grinding time established for

performing the assay was validated, since

the interval of the P80 obtained contains

the reference of the industrial practice.

The degree of liberation for each

milling test was analyzed and results

were 83.0%, 87.6%, 90.3% and 92.8%

188

for 20, 40, 60 and 80 minute milling,

respectively.

Figure 6 shows the graph relating

to the retained percentage on 0.074 mm,

the liberation degree and the energy consumption.

According with the speciication of

Votorantim the primary milling should

have 30% retained on 0.074mm for a

lotation of 93%. From the graph analysis,

the energy required for grinding, based

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

on the particle size distribution, for 30%

retained on 0.074 mm was 21 kWh/t. The

same veriication in accordance with the

liberation degree curve, showed an energy

consumption of 26.8 kWh/t for 93%.

The measurements made by both

parameters were very close, but for industrial practices, the highest value should be

adopted as the determining parameter, in

this case the liberation degree.

Alaine Moreira Imbelloni et al.

Figure 6

Relation between the energetic requirement and the % retained on 0,074 mm.

4. Conclusions

The results showed that the method

used to estimate the speciic energy consumption in industrial ball mills developed

by Donda is applicable for the primary

grinding stage of nickel ore with the typol-

ogy mentioned.

Industrial practice registers the

necessity of a 93.0% degree of liberation

to suit the subsequent lotation process.

For this demand, in practice 26.6 kW/t

has been consumed. When using Donda’s

method and adopting the liberation degree

as a parameter, the energy required was

26,8 kW/t, similar to the value obtained

in practice.

5. References

BERALDO, J.L. Moagem de minérios em moinhos tubulares. São Paulo: Edgar

Blücher, 1987. p. 1-47.

BOND F.C., 1961. Crushing and grinding calculations. Allis-Chaimers Publication,

No. 07R9235B (Revised).

BULATOVIC, S.M. Handbook of lotation reagents: chemistry, theory and practice.

Amsterdam: Elsevier Science & Tecnology Books, 2007. n.19 p. 401- 441.

CARVALHO, E. A., SILVA, A. O., JUNIOR, J. B. R., BRENNER, T. L. B. Níquel Mineração Serra da Fortaleza. Usinas de beneiciamento de minérios do Brasil.

Rio de Janeiro: CETEM, 2001. p 295 – 303.

CHAVES, A. P., PERES, A. E. C. Teoria e prática do tratamento de inérios – ritagem, peneiramento e moagem (3ª Ed.). São Paulo: Signus Editora, 2006. n.3.

DONDA, J. D. Um método para prever o consumo especíico de na remoagem de

concentrados de minérios de ferro em moinhos de bolas. Belo Horizonte: Universidade Federal de Minas Gerais, 2003. (Tese de Doutorado apresentada ao Curso

de Pós-Graduação em Engenharia Metalúrgica e de Minas - Área de concentração:

Tecnologia Mineral).

KRÜGER, F. L. Corpos moedores côncavos. Belo Horizonte: UFMG, 2004. (Tese de

Doutorado em Engenharia Metalurgica de de Minas).

MAN Y.T. A model-based scale-up procedure for wet, overlow ball mills. Brisbane,

Australia: The University of Queensland, 2000. (Ph.D Thesis).

WILLS, B. A., NAPIER-MUNN, T.J. Mineral processing technology. An introduction to the practical aspects of ore treatment and mineral recovery. (7ª, ed). Elsevier,

2006.

Received: 01April 2013 - Accepted: 08 May 2014.

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

189

Mining

Mineração

Nickel ore grinding energy

determination

Determinação energética da moagem do minério

de níquel

Alaine Moreira Imbelloni

Ma, Professora Assistente, CEFET

Araxá, Minas Gerais, Brasil

alaineimbeloni7@gmail.com

José Pedro Silva

Engenheiro Especialista, Samarco Mineração S/A,

Minas Gerais, Brasil

pedro@samarco.com

Carlos Alberto Pereira

Dr. Professor Associado, Universidade Federal de

Ouro Preto, Brasil

pereira@demin.ufop.br

Abstract

This study describes the application of an empirical method to estimate the energy consumption in laboratory of the primary grinding of nickel ore with a speciic

mineralogical texture. This method developed by Donda was previously used in iron

ore from the Iron Quadrangle (Minas Gerais, Brasil) with the same purpose. Through

the grinding test, performed under standard conditions and based on the degree of

liberation and percentage retained on 0.074 mm, it is possible to obtain the energy

consumption for grinding. The results mean a validation of the method with a good

approximation between industrial and laboratory values. In practice the energy consumption is 26.6 kWh/t and through Donda’s method, when using the liberation degree as a parameter, the energy found was 26.8 kWh/t.

keywords: Energy consumption, Nickel ore, Donda’s method

Resumo

Esse estudo descreve a aplicação de um método empírico para estimar, em laboratório, o consumo de energia de moagem primária do minério niquel com uma

textura mineralogica especíica. Esse método desenvolvido por Donda foi usado, anteriormente, em minério de ferro do Quadrilátero Ferrífero (Minas Gerais, Brasil), com

a mesma inalidade. Através do teste de moagem, realizado com condições padronizadas e baseado no grau de liberação e na percentagem retida em 0,074 mm, é possível

obter o consumo de energia de moagem. Os resultados signiicam uma validação do

método com uma boa aproximação entre valores industriais e laboratoriais. Na prática, o consumo de energia é 26,6 kWh/t e, através do método de Donda e usando o grau

de liberação como parâmetro, a energia encontrada foi de 26,8 kWh/t.

Palavras chave: Consumo energético, minério de níquel, metódo de Donda

1. Introduction

In mineral processing plants, the

comminution process is carried out in order to reduce particle size and “unlock”

the mineral species from the gangue,

enabling enrichment of the mineral

content to the desired level in subsequent

concentration processes (WILLS, 2006).

Over the years, various comminution theories were created and were only

concerned with the evaluation of the

relationship between applied energy and

particle reduction. Despite all advances

obtained in the knowledge of grinding, there is a gap about estimating the

speciic energy consumption. The laboratorial energy measurements require

complicated assembly and specialized

labor for the realization of tests. On

other hand, studies in industrial plants

require a large amount of material, take

a long time and have high costs.

Donda (2003) developed a method

to estimate grinding energy consumption

for ball mills using the iron ore concentrate from the Iron Ore Quadrangle

(Minas Gerais, Brazil). Its applicability

has been established for many years for

the re-grinding stage at Samarco Mineração S/A showing a good approximation between industrial and laboratorial

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

185

Nickel ore grinding energy determination

energy values with a range between 0.9

and 1.1 times the value of the s peciic

industrial energy consumption.

This method is an adaptation of the

methodology proposed by Bogren and

Wakeman, at the current Midland Research Center and consists of grindings

using different times with standardized

conditions for ball and ore charge, mill

speed and solid percentage, calculating

the absorbed power per tonne of grinding media through the Rowland equation

for a small mill (diameter until 0.76m).

The use of this method means a simpliication of the laboratory procedures as

being the differentiating factor, since the

tests can be performed in mills built with

minimum care and are not requiring

sophisticated equipment to measure the

energy in the laboratory (Von Krüger,

2004)

Studies about the nickel ore showed

that the liberation of nickel occurs in the

size of ines (0.074 mm) and requires

high power consumption in the primary

grinding. Then, considering the importance of controlling this parameter, this

study’s main goal was to verify the

applicability of the Donda’s method for

ine nickel ore.

was homogenized and quartered. The

grinding tests were performed in a ball

mill utilizing four different times (20,

40, 60 and 80 minutes) with standard

conditions as shown in Table 1. For each

test, the particle size analyses of the feed

and products were determined by wet

screening using Tyler sieves. Chemistry

analysis was performed with samples

of the ground products using optical

microscopy

2. Materials and methods

The experiments were done in the

Laboratory of Mineral Processing at the

University of Ouro Preto using a sample

of nickel ore from the mine of Fortaleza

de Minas belonging to Votorantim Metals Nickel S/A. The initial lot of material

Conditions for the Donda tests

Mill diameter (m)

0.3048

Mill length (m)

0.3048

Ball charge (kg)

30.578

% critical mill speed

70

% of solids

81

Ore charge (kg)

5.623

Media charge

Balls

Ball size distribution (diameter)

Staggered

Table 1

Pre-established conditions for the tests

(Donda, 2003).

(63 to 25 mm)

Using the Rowland equation

(Eq.1), the power was obtained by

multiplying the (kWb) value by the ball

load weight. The speciic energy was

obtained multiplying the power by the

milling time.

(Eq. 1)

Where:

kWb= Kilowatts per tonne of balls

D= Mill diameter inside lifters [m];

VP =Fraction of the mill volume oc-

cupied by the balls mill;

CS = Fraction of critical mill speed.

3. Results

Mineralogical analyses

The Table 2 shows the results of the

mineralogical analyses, which were done

based on the optical microscopy using the

product of the milling test for 60 minutes.

The samples used were composed mainly

of amphibole, pyrrhotite, chlorite, mag-

Mineral

%

Mineral

Amphibole

39

Carbonate

3

Pyrrhotite

20

Biotite

Trace

186

%

Chlorite

12

Chromite

Trace

Pentlandite

11

Pyrite

Trace

Talc + White

Mica/Sericite

6

Pyroxene

Trace

Magnetite

5

Goethite

Trace

Chalcopyrite

3

Ilmenite

Trace

Trace: < 1%

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

netite and pentlandite.

Table 2

Mineralogical analysis

Alaine Moreira Imbelloni et al.

According to the photomicrographs

obtained by optical microscopy with

transmitted light, it was possible to

determine that pentlandite is normally

associated with pyrrohotite as revealed

in Figure 1, which presented a lame of

pentlandite (PDT) in pyrrhotite (PYR).

The Figure 3 shows a pyrrhotite (PYR)

particle with pentlandite (PDT) lames

and a pentlandite (PDT) particle with

pyrrhotite (PYR) edges.

and pyrrhotite (PYR) particle associated

with pentlandite (PDT) as revealed in

Figure 4. For the product of grinding

performed during 80 minutes, note the

free particle composed of pentlandite

(PDT) in Figure 5.

Figure 1

grinding performed during 20 minutes

Figure 2

grinding performed during 40 minutes

After 60 minutes of grinding, it

was possible to notice the presence of a

particle liberated from pentlandite (PDT)

Figure 3

grinding performed during 60 minutes

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

187

Nickel ore grinding energy determination

Figure 4

grinding performed during 20 minutes

Granulometric analysis

Figure 6 shows the graph obtained

from the particle size distribution of

the feed and product for the grinding

tests. The results of P80, calculated as

a function of the test time at 20, 40, 60

and 80 minutes were 0.210 mm; 0.140

mm; 0.125 mm and 0.096 mm.

Figure 5

Particle size distribution

Liberation degree

Calculation of the liberation was

made by Gaudin, obtaining a particle

size equal to 0.125 mm, assuming there

is a variation of up to 3%. Therefore, the

sequence of grinding time established for

performing the assay was validated, since

the interval of the P80 obtained contains

the reference of the industrial practice.

The degree of liberation for each

milling test was analyzed and results

were 83.0%, 87.6%, 90.3% and 92.8%

188

for 20, 40, 60 and 80 minute milling,

respectively.

Figure 6 shows the graph relating

to the retained percentage on 0.074 mm,

the liberation degree and the energy consumption.

According with the speciication of

Votorantim the primary milling should

have 30% retained on 0.074mm for a

lotation of 93%. From the graph analysis,

the energy required for grinding, based

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

on the particle size distribution, for 30%

retained on 0.074 mm was 21 kWh/t. The

same veriication in accordance with the

liberation degree curve, showed an energy

consumption of 26.8 kWh/t for 93%.

The measurements made by both

parameters were very close, but for industrial practices, the highest value should be

adopted as the determining parameter, in

this case the liberation degree.

Alaine Moreira Imbelloni et al.

Figure 6

Relation between the energetic requirement and the % retained on 0,074 mm.

4. Conclusions

The results showed that the method

used to estimate the speciic energy consumption in industrial ball mills developed

by Donda is applicable for the primary

grinding stage of nickel ore with the typol-

ogy mentioned.

Industrial practice registers the

necessity of a 93.0% degree of liberation

to suit the subsequent lotation process.

For this demand, in practice 26.6 kW/t

has been consumed. When using Donda’s

method and adopting the liberation degree

as a parameter, the energy required was

26,8 kW/t, similar to the value obtained

in practice.

5. References

BERALDO, J.L. Moagem de minérios em moinhos tubulares. São Paulo: Edgar

Blücher, 1987. p. 1-47.

BOND F.C., 1961. Crushing and grinding calculations. Allis-Chaimers Publication,

No. 07R9235B (Revised).

BULATOVIC, S.M. Handbook of lotation reagents: chemistry, theory and practice.

Amsterdam: Elsevier Science & Tecnology Books, 2007. n.19 p. 401- 441.

CARVALHO, E. A., SILVA, A. O., JUNIOR, J. B. R., BRENNER, T. L. B. Níquel Mineração Serra da Fortaleza. Usinas de beneiciamento de minérios do Brasil.

Rio de Janeiro: CETEM, 2001. p 295 – 303.

CHAVES, A. P., PERES, A. E. C. Teoria e prática do tratamento de inérios – ritagem, peneiramento e moagem (3ª Ed.). São Paulo: Signus Editora, 2006. n.3.

DONDA, J. D. Um método para prever o consumo especíico de na remoagem de

concentrados de minérios de ferro em moinhos de bolas. Belo Horizonte: Universidade Federal de Minas Gerais, 2003. (Tese de Doutorado apresentada ao Curso

de Pós-Graduação em Engenharia Metalúrgica e de Minas - Área de concentração:

Tecnologia Mineral).

KRÜGER, F. L. Corpos moedores côncavos. Belo Horizonte: UFMG, 2004. (Tese de

Doutorado em Engenharia Metalurgica de de Minas).

MAN Y.T. A model-based scale-up procedure for wet, overlow ball mills. Brisbane,

Australia: The University of Queensland, 2000. (Ph.D Thesis).

WILLS, B. A., NAPIER-MUNN, T.J. Mineral processing technology. An introduction to the practical aspects of ore treatment and mineral recovery. (7ª, ed). Elsevier,

2006.

Received: 01April 2013 - Accepted: 08 May 2014.

REM: R. Esc. Minas, Ouro Preto, 67(2), 185-189, apr. jun. | 2014

189